The Journal of Textile and Clothing Science (JTCS) is a peer-reviewed (refereed) journal. Which is aimed at providing the platform to exchange information pertaining to all sectors of textile and the clothing industry among researchers, textile technocrats, fashion designers and industry experts. The journal focuses on scientific, technical, economical, managerial and all other aspects of textile activity at theoretical and experimental level. JTCS is aimed at publishing original research articles, review papers, short communications, and letters to the editor and book reviews catering the needs of both industry and academia.
Journal of Textile and Clothing Science questions gotten by the technologist from the purchasers are connected in somehow, to the solace parts of the substrates and thus normal intensions are traveling toward assist enhancements. Numerous specialists are growing new crude material which improve the durability and serviceability of fabric. Woven textiles are intended to meet the necessities of their end utilize. Their quality, thickness, extensibility, porosity and durability can be differed and rely on upon the weave utilized, the string dispersing, that is the quantity of strings per centimeter, and the crude materials, structure (fiber or staple), direct thickness and curve components of the twist and weft yarns. From woven fabrics, higher qualities and more prominent strength can be gotten than from whatever other fabric structure utilizing interweaved yarns. Structures can likewise be fluctuated to create fabrics with broadly extraordinary properties in the twist and weft headings. The property of any fabric created relies on upon the constituent strands material, yarns and the fabric structure and how every one of these variables collaborate with each other. A definitive point of any clothing fabric is to fulfill the wearer and make him feel great. Consequently, with regards to above it is worth to examine the solace properties of various woven fabrics. 2. Methodology This investigation focuses on the various comfort, durability and serviceability characteristics of different woven structures, woven using double yarn with 2:1 setting ratio on shuttle less weaving machine. Total 7 different types of weaves viz. plain, 2/2 matt, warp rib, 3/1 twill, herringbone twill, satin and crepe were studied to investigate the comfort and other properties. Cotton yarn was used in warp for all Sr. No. the effect of weft material on fabric properties. Finishing treatments like singeing, desizing, mercerizing, bleaching and resin finishing were carried out on fabric. All the fabric specimens in grey as well as in finished condition were tested in standard atmospheric conditions for properties like crease recovery, abrasion resistance, and tearing strength. After testing obtained results were analyzed using Minitab statistical software. 2.1 Materials 2.1.1 Warp and Weft yarns 100% cotton yarn was used as warp for all the fabric specimens and the same yarn was used as one of the weft. 100% cotton (same yarn that was used in warp), 80:20 blended cotton/polyester and 120 denier cot look polyester multifilament yarn were used in weft. Raymond Zambaiti LTD. Kagal provided 100% cotton and P/C blended yarn and cot look polyester yarn was procured from Reliance, Ichalkaranji. All weft yarns were selected such that their linear density in nearly equal. Characteristics of these yarns were tabulated in table 1. 2.1.2 Chemicals Chemicals like Alpha amylase enzyme, wetting agent, sequestering agent and deformer were used for desizing of fabric. NaOH was used for mercerization. H2O2, peroxide stabilizer and soda ash for were used for bleaching process and Saralink ULF Resin, Acetic Acid, Extra soft Silicon softener, Expocil CEL Antisliping agent, Macl2, Sarasoft EP Tear improver and JET-B Wetting agent were used for finishing treatment of fabric. Raymond Zambaiti LTD. Kagal provided all these chemicals. 2.2 Method Table 1: Characteristics of yarns Yarn Characteristics Cotton Cotton/Polyester Polyester 1 Count (Ne) 42.14 42.3 44.29 (120D) 2 Tensile Strength (g/tex) 16.82 24.65 26.37 3 Elongation (%) 3.45 7.57 14.95 4 Hairiness Index 3.1 4.54 - 5 Unevenness (U %) 7.63 10.82 - 6 Twist Per Inch 27.2 22.3 - weaves. Cotton, polyester/cotton and cot look polyester yarn were used in weft to investigate As mentioned earlier 100% Raymond Zambaiti LTD. Kagal provided cotton and P/C 4 Volume: 01 Issue: 01 | January-March-2018, www.jtcsonline.com
Journal of Textile and Clothing Science Table 2: Specification of weaving machine blended yarn and cot look polyester yarn was procured from Reliance, Ichalkaranji. All these yarns were double yarns. After procurement, all yarns were tested for different properties such as linear density (count), single yarn strength, hairiness, unevenness and level of twist. After testing, fabric with double yarn in warp and weft and ends/picks having 2:1 set ratio was manufactured on shuttle less weaving machine with different weaves. The gray fabric was processed and finished. Testing of gray as well as finished fabric was carried to find out different fabric properties. specimens were manufactured. After manufacturing the fabrics, finishing treatment was given. In brief, finishing treatment was (a) Plain (b) 2/2 Matt 2.2.1 Fabric Manufacturing Weaver’s beams were prepared on Suzuki 4 NAS-M6 warping machine running at 800 mpm. After getting weavers beam, fabric samples with double yarn in warp and weft having 2:1 set ratio i.e. 120 ends and 60 picks were manufactured on Sliver Vamatex rapier weaving machine. The variable factors were fabric weave and weft yarn. Fabrics with seven different type of weaves were woven on rapier weaving machine. Specification of machine were shown in table 2. Specification Loom type Model Details Flexible Rapier Sliver Vamatex, Itema (c) 2/2 Warp Rib (e) 2/2 Herringbone Twill (d) 3/1 Twill (f) 4 End Satin Let off Speed Electronic 400 rpm Total ends 8700 Reed space 178 cm Reed count 24.4 No. of shaft 8 Colours feed in weft 1 No. of heald frames 8 Weaves include the basic weaves like plain, 3/1 twill and satin along with their derivatives like 2/2 matt, warp rib, herringbone twill and crepe. Fig. 1 depicts the different fabric structures, which were woven. The 100% cotton yarn was used in warp for all the fabric specimens. 100% cotton yarn, 80:20 blended cotton/polyester yarn and cot look polyester multifilament yarn was used as weft for all the weaves. Each weave was woven using all the three type of weft yarns separately. With every possible combination, 21 fabric (g) Crepe Figure 1: Fabric structure /weaves explained in following points (see 3.3.2). All the grey as well as finished fabric specimens were characterized for different properties. All the fabric samples were manufactured in M/S Raymond Zambaiti LTD. Kagal. 2.2.2 Fabric Processing After manufacturing the fabric with all possible combination. All the manufactured fabric samples were subjected to finishing treatments like singeing, mercerizing, bleaching and resin finishing. Singeing was done by gas singing method at 80 m/min with 12 bar flame intensity. After singeing, scouring of fabric was carried out. Scoured and dried samples were Volume: 01 Issue: 01 | January-March-2018, www.jtcsonline.com 5